Assessment and comparison of retention of zirconia copings luted with different cements onto zirconia and titanium abutments: An in vitro study Neelima Sreekumar Menon, G. P. Surendra Kumar, K. R. Jnanadev, C. L. Satish Babu, Shilpa Shetty Department of Prosthodontics, VS Dental College and Hospital, Bengaluru, Karnataka, India
Aim: The purpose of this in vitro study was to assess and compare the retention of zirconia copings luted with different luting agents onto zirconia and titanium abutments. Materials and Methods: Titanium and zirconia abutments were torqued at 35 N/cm onto implant analogs. The samples were divided into two groups: Group A consisted of four titanium abutments and 32 zirconia copings and Group B consisted of four zirconia abutments and 32 zirconia copings and four luting agents were used. The cemented copings were subjected to tensile dislodgement forces and subjected to ANOVA test. Results: Zirconia abutments recorded a higher mean force compared to titanium. Among the luting agents, resin cement recorded the highest mean force followed by zinc phosphate, glass ionomer, and noneugenol zinc oxide cement, respectively. Conclusion: Highest mean retention was recorded for zirconia implant abutments compared to titanium abutments when luted with zirconia copings. Key Words: Titanium abutment, zirconia abutment, zirconia copings
Address for correspondence: Dr. Neelima Sreekumar Menon, Department of Prosthodontics, VS Dental College and Hospital, K R Road, VV Puram, Bengaluru, Karnataka, India. E‑mail: [email protected]
Received: 4th February, 2015, Accepted: 19th November, 2015
Main goals of restorations in modern dentistry are optimal function and esthetics. The options for restoring edentulous areas have changed dramatically with the introduction of endosseous dental implants. Clinical decisions are not only limited to the selection of the type of implant but also the type of abutment and cement used. Initially, implant‑supported prostheses were exclusively retained by screws, but with the development of new implant systems Access this article online Quick Response Code:
and rehabilitation techniques cement retained prostheses have become popular treatment option. Cement‑retained superstructures over the implant abutments assure passive fit because of the cement layer between the framework and abutment. Other advantages of cement‑retained implant restorations include improved direction of load, enhanced esthetics, easy access, reduced fabrication cost and time, simplified restorative procedures, and optimum occlusion excluding the interference of screw access openings. This is an open access article distributed under the terms of the Creative Commons Attribution‑NonCommercial‑ShareAlike 3.0 License, which allows others to remix, tweak, and build upon the work non‑commercially, as long as the author is credited and the new creations are licensed under the identical terms. For reprints contact: [email protected]
How to cite this article: Menon NS, Surendra Kumar GP, Jnanadev KR, Satish Babu CL, Shetty S. Assessment and comparison of retention of zirconia copings luted with different cements onto zirconia and titanium abutments: An in vitro study. J Indian Prosthodont Soc 2016;16:136-41.
© 2016 The Journal of Indian Prosthodontic Society | Published by Wolters Kluwer - Medknow
Menon, et al.: Retention of zirconia copings using different cements
Limitations associated with the cement‑retained implant restorations include low profile retention, when there is limited interarch space, retrievability, and presence of cement in the sulcus. Commercially, pure titanium has been widely used as an abutment material in implant therapy because of its well‑documented biocompatibility and mechanical properties. Recently, zirconia implant abutment materials have gained popularity because of their better fracture resistance and superior optical properties over titanium. Selection of luting agent is very important for cement‑retained implant prostheses and it is largely dependent on operator preference, convenience, and manufacturer recommendations. Ideal luting agent should be strong enough to retain the restorations yet weak enough so that restorations can be removed easily if required. The aim of this study was to assess and compare the retentive strengths of different classes of luting agents used to cement zirconia copings to titanium and zirconia implant abutments.
Figure 1: Titanium abutment mounted on acrylic resin blocks
MATERIALS AND METHODS
Materials used in the present study included eight implant analogs (Collagen Meniscus Implant [CMI]), four titanium [Figure 1] abutments (CMI, hexed abutment), four zirconia abutments [Figure 2], and 64 zirconia copings (Lava, Zirconia 3M ESPE) [Figures 3 and 4]. The luting agents used were resin cement (Calibra‑Densply), glass ionomer (GC gold label luting and lining cement), zinc phosphate (Harvard Cement), and zinc oxide noneugenol (Rely X™ Temp NE) cements.
Figure 2: Zirconia abutment mounted on acrylic resin blocks
Fabrication of resin blocks and emdedding specimen
Eight implant analogs (CMI) were embedded in acrylic resin blocks, titanium and zirconia abutments were torqued into implant analogs. Acrylic resin blocks were fabricated to facilitate mounting the specimen on tensile strength testing machine. Implant analogs were embedded into acrylic block. Abutments were torqued onto implant analogs. An 8 mm diameter hole was drilled at the end of acrylic block to facilitate mounting the specimen on tensile testing machine. A single operator prepared all eight resin blocks and implant analogs were embedded, and abutments were torqued at 35 N/cm. Both zirconia and titanium abutments used in the study were of 7.4 mm in height with 8° convergence angle and 5.8 mm in diameter. Fabrication of zirconia copings
Samples were divided into two groups. Group A consisted of four titanium abutments and 32 zirconia copings. Group B consisted of four zirconia abutments and 32 copings. Resin pattern were made for zirconia copings; an extension was made on the occlusal surface of each coping parallel to long axis of
Figure 3: Group A consisting of four titanium abutments and 32 zirconia copings
the tooth to serve as a connector to the tensile strength testing machine. zirconia copings thus designed were milled with computer aided designing – computer aided manufacturing unit.
The Journal of Indian Prosthodontic Society | Apr-Jun 2016 | Vol 16 | Issue 2 137
Menon, et al.: Retention of zirconia copings using different cements
Cementation of copings
Both Groups A and B were randomly divided into four groups each comprising specimens Groups 1‑4. Zirconia copings in Groups A1 and B1 were cemented with glass ionomer (GC gold label luting and lining cement) cement, Groups A2 and B2 were cemented with resin cement (Calibra‑Densply), Groups A3 and B3 were cemented with zinc oxide noneugenol cement (Rely X™ Temp NE), and Groups A4 and B4 were cemented with zinc phosphate cement (Harvard Cement). Each coping of all groups was sandblasted with 50 µm aluminum oxide before cementation. Cements were mixed according to the manufacturer’s instructions and were applied in a thin layer to the inner axial walls of the crown. Each coping was seated on its perspective abutment with firm finger pressure and then placed under a 10 kg weight for 5 min and cementation was carried out [Figure 5]. Excess cement was removed with an explorer. Thermocycling and tensile testing
Specimens were stored at room temperature for 24 h and immersed in artificial saliva for 7 days, after which specimens were thermo cycled 100 times between 5°C and 55°C with
a dwell time of 10 s, dried and subjected to retention test. The cemented copings were subjected to tensile dislodgement forces using crosshead speed of 0.5 mm/min until cement failure occurred [Figures 6‑8]. The same abutment was used with each of the coping and four cements were evaluated. Abutments were cleaned with a plastic explorer. Abutments were immersed in an ultrasonic cleaner for 15 min and re‑used. RESULTS
Results obtained from the retention test were statistically analyzed using factorial ANOVA test. Among the cements, the highest mean force was recorded in resin cement followed by zinc phosphate, glass ionomer, and noneugenol zinc oxide, respectively. The difference in mean force recorded between them was found to be statistically significant (P